DENTURE BASE• Denture :- they are prosthetic device constructed to replace the missing teeth which are supported by surrounding hard & soft tissues• Two types of denture:• COMPLETE DENTURE• REMOVBLE PARTIAL DENTURE• DENTURE BASE -fabricated using common polymer
• Commonly used denture polymers: Individual processing system Polymerization technique
GENERAL TECHNIQUE1. Fabrication of accurate impression of the associated arch2. Dental arch generated3. Record base is fabricated on the cast4. Wax added to record base & teeth is positioned in wax5. Denture flask –tooth arrangement is encased in investing medium6. Denture flask is opened & wax is eliminated7. After through cleansing –a resin denture base material is introduced into the mold cavity denture base resin is polymerized8. Denture is recovered &prepared for insertion
ACRYLIC RESINS• Denture base fabricated with POLY (METHYL METHACRYLATE) resins• Pure PMMA –colorless ,transparent solid• Advantage PMMA as denture base material is the relative ease with which it an be processed .• PMMA supplied –powder& liquid system• powder-prepolymerized PMMA resin• Liquid-non polymerized methyl methacrylate• Liquid & powder mixed in a proper proportions- workable mass is formed .
HEAT –ACTIVATED DENTURE BASE• Used in fabrication of all denture base• Thermal energy required for polymerization –water bath or microwave oven• COMPOSITION• PMMA –powder & liquid• Powder –prepolymerized spheres of PMMA & small amount of benzoyl peroxide(INITIATOR)• Liquid –predominantly non polymerized methyl methacrylate with small amount of hydroquinone(INHIBITOR)• Cross linking agent is added to liquid
methylmeth crosslinked Glycol acrylate polymethyl dimethacrylate methacrylate STORAGE- generally recommended specific temparature & time limits for storage of heat activated denture base
COMPRESSION MOLDING TECHNIQUEHeat activated denture base are shaped via compression molding 1) The master cast and the wax dentures are placed in the flask, to insure that the cast fit in the flask2.The Inner surface of the flask iscoated with Vaseline, while thebase of the cast is painted withseparating medium (cold moldseal). To prevent the investmentmaterial (plaster of Paris) fromattaching to the cast
3) The first layer of gypsuminvestment is poured in thelowerhalf and the cast is placed on topof the investment4) After the set of the first gypsuminvestment layer, a plasterseparating medium is painted onit, to prevent the sticking of thesecond layer of gypsuminvestment to the first layer.
5) A mix of dental stone is placed over the surface of the teeth in the invested trial denture , which is referred to as coring.6)The upper half of the flaskis put inplace, then the second mix ofgypsum investment is placedonthe first layer and covers thewax, denture base and teeth.
7) Before the second layer setsthe lidor flask cover is put in place andtapped to sit properly allowingthe excess gypsum to flow out ofthe holes in the lid.2- Wax elimination:After the complete set of the gypsumthe flask is ready for the next stepwhich is "Waxelimination", in which the flask isplaced in boiling water for 4 to 6minutes. Then it isremoved from the water and opened.Then the wax is washed away withboiling water. Afterthat the mold is washed with boilingwater containing detergent, then finallywashing it withclean boiling water.
3- Mixing:Acrylic resin dough is made by mixing the powder (polymer) and liquid (monomer)to form dough which is packed into a gypsum mold for curing. The ratio of powderto liquid is important since it controls the workability of the mix as well as thedimensional changes on setting . The mixing should be done in a clean jar whichshould be covered to prevent evaporation of the monomer.:4- Packing:It should be done when the mixture reaches dough stage, as the dough is rolled into arod-like form and placed in the upper half of the flask then a polyethelen (nylon sheet) isplaced over the dough in the upper half and then the two halves of the flask are closed untilthey are almost in approximation, this is done to spread the dough evenly throughout themold. 5- Curing: It is polymerization of the hot cure acrylic to produce the final denture. The mater is cured by heating in a water bath; pressure is applied during curing reasons: 1- To decrease the effect of thermal expansion. 2- To decrease the polymerization shrinkage. 3- To increase the evaporation of monomer thus decreases porosity
SELECTION & APPLICATION OFSEPARATING MEDIA• It must prevent direct contact between the denture base resin & mold surface• Failure to place appropriate separating medium leads to :• it may effect the polymerization rate as well as optical & physical properties of the denture base• Portions of the investing medium may become fused to denture base• Widely accepted method : thin sheet of tin foil ,painting –on separating media• Commonly used separating medium – water soluble alginate solutions
POLYMER-MONOMER RATIO• Powder & liquid are mixed in proper proportions• Polymer monomer ratio – 3:1 by volume• Excess monomer – increase polymerization shrinkage
POLYMER –MONOMER INTERACTION• When monomer &polymer are mixed in proper proportion –workable mass is formed• Workable mass result in 5 stages:I. SANDY-coarse or grainyII. STRINGY-stringiness or stickiness when material is touchedIII. DOUGHLIKE- ideal for compression moldingIV. RUBBERY or ELASTIC-mass rebounds when compressed or stretchedV. STIFF-resistant to mechanical deformation
• DOUGH FORMING TIME• ADA specification- less than 40 min from start of mix• Working time• ADA specification – 5mins ,dough to remain moldable• Extended by refrigeration
PACKING• The placement & adaptation of denture base resin within mold cavity is termed PACKING• OVERPACKING(placement of too much material)- excessive thickness & malpositioning of teeth• UNDERPACKING(use of too little material)- leads to denture base porosity
• TO MINIMIZE OVERPAKING & UNDERPAKING:1. Performed in doughlike stage2. Rolled in ropelike form& bent in horseshoe shape3. Polyethylene sheet placed over the resin4. Designed pressed, until flask is closed5. Polyethylene sheet is removed6. Using gently rounded instrument , excess flash is removed
INJECTION MOLDING TECHNIQUE1. Denture base fabricated by specially designed flask2. One half of flask is filled with freshly dental stone &master cast is settled in the stone3. Dental stone is allowed to set , sprues are attached to the wax denture base4. Wax elimination5. Flask is placed into a carrier6. After completion of these steps the resin is injected in the moldcavity7.Powder &liquid mixture is used ,resin is mixed & introduced in roomTemparature8.Flask is placed in boiling water bath for polymerization of denture base resin(as it polymerizes additional resin is introduced into the mold cavity , this effects polymerization shrinkage)8. The denture is recovered , adjusted,finished ,polished
ADVANTAGE: denture base fabricated by injection molding provide improved clinical accuracy
POLYMERIZATION PROCEEDURE• Denture base resin generally contain benzoyl peroxide• When heated above 60 degree , molecules of benzoyl peroxide decompose to yield electrically neutral species containing unpaired electrons .These species are termed as FREE RADICALS• DECOMPOSITION of benzoyl peroxide molecules yields free radicals which initiate the chain growth,benzoyl peroxide is termed as initiator• Heat is termed as the activator• Denture base carrier heat applied to resin by immersing flask in a water bath
TEMPARATURE RISE• Polymerization of denture base resin is exothermic• Resin occupies a position in centre of the mold->heat penetration takes longer time• Temp of resin exceeds the boiling point of monomer(100.8 C)• INTERNAL POROSITY• Boiling yields porosity within complete denture base• Heat is disipated ,surface tension of resin does not reach the boiling point of monomer ,because resin is a poor thermal conductor• Peak temp of this resin may rise above the boiling point of monomer, cause unreacted monomer• Unreacted monomer produce porosity within the processed denture
POLYMERISATION VIA MICROWAVE• PMMA –using microwave energy• Formulated resin & non metallic flask is used• Conventional microwave oven –used to supply thermal energy• Advantage: polymerization is accomplished with speed
CHEMICALLY ACTIVATED DENTURE BASE RESIN • Induce the denture base polymerisation • Does not require thermal energy, made in room temparature • chemically activated resins also referred-cold curing ,self curing or autopolymerizing resins • COMPOSITION • liquid(monomer) - Addition of tertiary amine like dimethyl-para-toluidine • Tertiary amines causes decomposition of benzoyl peroxide • Mold preparation &resin packing is same as heat activated resin
DIFFERENCE BETWEEN HEATACTIVATED & CHEMICALLY ACTIVATED• Benzoyl peroxide is divided to yield free radical• Degree of polymerization is not as complete as heat activated• DISADVANTAGE:• The unreacted monomer cause 2 major difficulties:• It acts as plasticizer –decreased transverse strength of denture resin• Residual monomer serve as potential tissue irritant• ADVANTAGE:• Less shrinkage than heat activated resins-gives greater dimensional accuracy• Color stability is inferior to the color stability of heat activated resins• Working time is shorter than heat activated materials• Rate of polymerization process decreases- resin remains in dough stage for extended period , working time is increased
FLUID RESIN TECHNIQUE• Pourable chemical activated resin• Resin is supplied in form of powder & liquid components• Very low viscosity resin• Completed tooth arrangement positioned in a fluid resin flask• Tooth arrangement is removed from irreversible hydrocolloid• Preparation of sprues and vents for resin• Repositioning of posterior teeth & master cast• Resin is poured into the mold cavity & allowed to polymerize• Flask is kept in pressureised chamber for 30 -45 mins• Recovery of complete denture prosthesisADVANTAGE:1. Improved adaptation to underlying soft tissue2. Decreased probability of damage to prosthetic teeth &denture bases during flasking3. Reduced material cost4. Simplification of flasking ,deflasking &finishing procedureDISADVANTAGE:1. Noticeable shifting of prosthetic teeth during processing2. Air entrapment within the denture base material3. Poor bonding between the denture base material &acrylic resin teeth4. Technique sensitivity
LIGHT ACTIVATED DENTURE BASE RESINS• Composite matrix of urethane dimethacrylate ,microfine silica ,&high molecular weight acrylic resin monomer• Activator –visible light• Initiator –camphorquinone• Supplied in sheet &rope form packed in light proof pouches• light activated resin cannot be flasked in conventional manner• Opaque investing media provides the passage of light• Teeth is arranged & the denture base sculpted using light activated resin• Denture base is placed into a light chamber &polymerized
PHYSICAL PROPERTIES OF DENTUREBASE RESINS• Critical to fit & function of removable dental prostheses• Characteristics-polymerization ,shrinkage ,porosity ,water absorption ,solubility ,processing stresses & crazing